Local structure of LiNiO2 studied by neutron diffraction

PHYSICAL REVIEW B 71, 064410 2005**Local** **structure** **of** LiNiO 2 **studied** **by** **neutron** **diffraction**J.-H. Chung*Department **of** Materials Science and Engineering and Laboratory for Research on the Structure **of** the Matter,University **of** Pennsylvania, Philadelphia, Pennsylvania 19104, USATh. Pr**of**fenLujan Center, Los Alamos National Laboratory, Los Alamos, New Mexico 87545, USAS. ShamotoNeutron Science Research Center, JAERI, Tokai, Ibaraki, 319-1195, JapanA. M. GhorayebLaboratoire Matériaux et Microélectronique de Provence, CNRS UMR 6137, Université d’Aix-Marseille III, Case 142,13397 Marseille Cedex 20, FranceL. CroguennecInstitut de Chimie de la Matière Condensée de Bordeaux, CNRS, 33608 Pessac Cedex, FranceW. TianDepartment **of** Physics and Astronomy, University **of** Tennessee, Knoxville, Tennessee 37996, USAB. C. Sales, R. Jin, and D. MandrusOak Ridge National Laboratory, Oak Ridge, Tennessee 37831, USAand Department **of** Physics and Astronomy, University **of** Tennessee, Knoxville, Tennessee 37996, USAT. EgamiDepartment **of** Materials Science and Engineering and Department **of** Physics and Astronomy,University **of** Tennessee, Knoxville, Tennessee 37996, USAand Oak Ridge National Laboratory, Oak Ridge, Tennessee 37831, USAReceived 25 May 2004; revised manuscript received 8 November 2004; published 22 February 2005The nature **of** the magnetic state **of** LiNiO 2 has been controversial. In this compound Ni spins S=1/2 forma triangular lattice with the possibility **of** magnetic frustration, but the exact state **of** spin correlation has not yetbeen known in spite **of** the extensive research work. A factor that complicates understanding **of** the magneticstate is the orbital state **of** Ni 3+ which is a Jahn-Teller JT ion. While there is no signature **of** long-rangeJahn-Teller distortion, local JT distortion has been suspected. We have performed **neutron** **diffraction** andatomic pair-density function analyses up to unprecedented large distances to discover a number **of** unusualfeatures, such as anomalous peak broadening, local JT distortion, sharp oxygen-oxygen distance correlations,and inverted temperature dependence **of** medium range correlation. These observations are best explained **by**local orbital ordering **of** Ni 3+ ions into three sublattices. This orbital ordering, however, cannot develop intolong-range order because **of** the strain field it generates, and domains **of** about 10 nm in size are formed.Domains are susceptible to random pinning **by** impurities site disorder resulting in the loss **of** structurallong-range order. We suggest that this local orbital ordering is the basis for the complex magnetic propertiesobserved in this compound.DOI: 10.1103/PhysRevB.71.064410PACS numbers: 61.12.Ld, 71.27.a, 71.70.EjI. INTRODUCTIONFrustrated magnetism is a subject **of** considerable researchattention at present, not only because it is an interesting phenomenon,but also because frustrated spin systems are highlysusceptible to perturbations and could lead to novel phenomenathrough interplay with other forces. A classic example **of**frustrated spin systems is antiferromagnetic Ising spins forminga triangle, where the third spin cannot be in a minimumenergy configuration with both neighbors simultaneously. Inthe two-dimensional triangular lattice there are manifolds **of**possible ground states leading to the frustration **of** the wholesystem. In LiNiO 2 Ni 3+ spins form two-dimensional triangularnetworks separated **by** Li layers, which provide a groundfor geometrical frustration. It has earlier been suggested 1 as acandidate system for the exotic resonant valence bond RVBstate 2 to occur. While the likelihood **of** the RVB state in thiscompound appears to be in doubt, a number **of** competingproposals on possible magnetic ground states have been suggested,including two-dimensional 2D Ising ferromagnet, 3frustrated antiferromagnet, 4–7 spin glass, 8–11 quantum disor-1098-0121/2005/716/06441011/$23.00064410-1©2005 The American Physical Society

CHUNG et al.FIG. 1. a A side view **of** LiNiO 2 **structure** R3¯m revealingstacks **of** NiO 2 slabs and Li layers. The thin solid lines connectingfour Ni sites denote the boundary **of** a unit cell. b A top view **of** aNiO 2 slab showing the network **of** edge-shared octahedra. At theright bottom corner, the threefold arrangement **of** Ni 3d 2 −r 2 /3 =x, y, orz orbitals is also shown.PHYSICAL REVIEW B 71, 064410 2005dered state, 12 etc., and the question is still wide open.Whereas these studies were restricted to low-temperaturestudies, a recent work 13 extended the measurement to hightemperatures and proposed the possibility **of** orbital frustration,which would have significant impact on the magneticproperties. This proposal was based on the observation **of**anomalies in spin susceptibility at two distinct temperaturescales, at 10 and at 400 K, which they interpreted as originatingfrom spin interaction and orbital interaction, respectively.Ni 3+ has d 7 configuration that splits into t 6 12g and e g**by** the octahedral crystal field, so that it is a Jahn-Teller ion.They surmised that the local Jahn-Teller distortion 14,15 maybe responsible for the large energy scale that produces theanomaly around 400 K. The primary purpose **of** the presentwork is to determine the orbital state **of** this compoundthrough **neutron** **diffraction**, analyzed both in real and reciprocalspaces. The knowledge obtained in this work shouldfacilitate understanding **of** the magnetic interactions in thissystem.LiNiO 2 has a layered **structure** made **of** stacks **of** NiO 2layers with intercalating Li layers Fig. 1a. Figure 1bshows the top view **of** the NiO 2 layer or slab with triangularsymmetry. The building block **of** the NiO 2 layer is a NiO 6octahedron, as is commonly found in transition metal oxides.Unlike the cuprates and manganites that have a corner-sharednetwork **of** octahedra, LiNiO 2 has an edge-shared network **of**NiO 6 octahedra. The corner-shared network **of** MO 6 octahedrahas linear M-O-M bonds, which can easily be buckled.However, in the edge-shared network two M ions are connected**by** two oxygen ions, so the network is much morerigid, and this has a major implication as we discuss below.Since Ni 3+ is a strong Jahn-Teller JT ion, a topologicallyequivalent compound NaNiO 2 shows collective collinear JTdistortion with variation in the NiuO distance as much as6%. 16,17 Since such a collective distortion has not been observedfor LiNiO 2 , it has **of**ten been assumed that in LiNiO 2the JT orbitals are randomly oriented. 14,18 Structurally, however,the random orientation **of** the JT orbital in the rigidtriangular network is very unlikely. There is also a speculationthat the JT orbitals in LiNiO 2 order collinearly as inNaNiO 2 but their collective orientations split into nanodomainsdue to impurities. The purpose **of** the present workis to determine the local **structure** **of** LiNiO 2 **by** **neutron** **diffraction**and to investigate the possible connection betweenthe observed magnetic property and the underlying orbitalstate. We show that the orientations **of** JT orbitals in LiNiO 2are neither random nor collinear, but instead they form anordered pattern that is compatible with triangular symmetry.The orbital ordering, however, is prevented from developinginto long-range order because **of** the strain field it generates,and domains **of** about 10 nm in size are formed. We suggestthat this local orbital ordering is the basis for the complexmagnetic properties observed in this compound.II. EXPERIMENTAL METHODSTwo different powder samples **of** LiNiO 2 were used inthis study. One sample 1 was prepared following the proceduredescribed **by** Rougier et al., 14 while the other sample2 followed the procedure **by** Bianchi et al. 19 LiNiO 2 tends tohave Li and O vacancies which make it an ionic conductor. 9Special care was taken to limit these vacancies to below0.1%. Neutron powder **diffraction** pr**of**iles were obtained **by**the NPDF diffractometer at Manuel Lujan Neutron ScatteringCenter **of** Los Alamos National Laboratory. NPDF wasrecently upgraded **by** adding expanded backscattering detectorbanks with large arrays **of** 3 He position sensitive detectorsthat increased the data collection rate **by** more than a factor**of** 5. 20 A powder sample was sealed in a vanadium can withHe heat exchange gas and placed in a cry**of**urnace. The measurementswere made at various temperatures between 10and 585 K. At each temperature data were collected roughlyfor 4 h, which produced excellent statistics suitable for bothreciprocal space Rietveld analysis and real space atomic pairdensityfunction PDF analysis. Additional backgroundmeasurements were also made in order to obtain the **structure**functions purely from samples for the real space PDF analysis.The reciprocal space Rietveld refinement analysis wasperformed with the GSAS package. 21 Only the histogramsfrom the 90°-detector banks were chosen for the refinement,since the peak pr**of**ile from conventional tube detectors canbe precisely fitted with well-known pseudo-Voigt functions.It was assumed that the major defect is Ni Li , so the formula isLi 1−x Ni x NiO 2 . Under this assumption, the defect concentration**of** sample 1 was estimated to be x=0.0235±0.004 fromthe Rietveld refinement. The sample 2 had a higher defectconcentration x=0.0388. We note that we also have triedother possibilities, such as Li 1−x Ni x Ni 1−x Li x O 2 orLi 1−x Ni x Ni 1−y Li y O 2 . Naturally, the latter gave the bestagreement factor, since it has higher number **of** refinable parameters.However, it is reasonable to assume that the majorpoint defect in this sample is the Ni Li , since Li + ion is toolarge to enter the Ni 3+ site. In any case, the estimated defectconcentration was well below 3% for the sample 1.The atomic pair density function PDF which is the Fouriertransformation **of** the **neutron** **diffraction** pr**of**ile, was calculated**by** the following equation:064410-2

LOCAL STRUCTURE OF LiNiO 2 STUDIED BY…PHYSICAL REVIEW B 71, 064410 2005Gr =4r 0 gr −1 QSQ −1sinQrdQ,=0where gr is the pair distribution function, 0 is the averageatomic density, and SQ is the normalized **structure** functiondetermined from the **diffraction** intensity. 22 The **diffraction**data were processed using the PDFGETN program. 23 Since thesignal to noise ratio deteriorates quickly with increasing Q, itis advantageous to introduce cut**of**f in Q, which was chosento be 35–40 Å −1 in this study. At the same time a theoreticalpair distribution function can be calculated **by** the followingformula, which serves as the basis for the refinement:G calc r = 1rN i,jb ib jb 2r − r ij −4 0 ,where b i and r ij are the scattering length **of** ith atom and thedistance between ith and jth atom, respectively, and N is thenumber **of** atoms. In real data, the distance correlations expressedas functions in Eq. 2 are broadened due to thermalfluctuations. This effect is described **by** convolution withGaussians with certain widths determined **by** the De**by**e-Waller factors.The PDF has traditionally been used for the analysis **of**local **structure** up to 10 Å or so. However, we note that inthis work we determined and analyzed the PDFs up to verylarge distances as have never been done before. The accuracy**of** the PDF in terms **of** distances is related to the resolution inQ. Just as the real space uncertainty due to lattice vibrationbecomes the multiplicative De**by**e-Waller factor upon Fouriertransform, Q translates to an envelope function for thePDF. 22 In a time-**of**-flight spectrometer used for pulsed **neutron**sQ is proportional to Q and deteriorates at high Q,limiting the range **of** the PDF in distance. The NPDF spectrometerhas a very high resolution **of** Q/Q=0.0015 atbackscattering, allowing the PDF to be determined accuratelyup to very large distances. 20 This enables seamlessstructural characterization ranging continuously from the local**structure** to the medium-range and long-range **structure**.For the purpose **of** comparison, especially for the long-rangePDF peaks, we also have measured the **neutron** **diffraction** **of**LiVO 2 and Na 0.75 CoO 2 . The former has exactly the samecrystal **structure** and space group as far as average **structure**is concerned, while the latter has the space group P6 3 /mmcbut a similar triangular symmetry with edge-shared octahedra.The measurements **of** these compounds were done at 12and 290 K using a closed cycle refrigerator.III. EXPERIMENTAL RESULTSA. Rietveld refinement **of** **neutron** **diffraction**For the analysis **of** the structural change with temperature,we began with refining the **neutron**-**diffraction** data with theRietveld method at a temperature in the middle **of** the range**studied**, 335 K, and proceeded **by** applying the obtained **diffraction**peak pr**of**ile parameters for the data at different temperatures.The space group **of** LiNiO 2 was initially assumed12FIG. 2. The Rietveld refinement analysis **of** the **neutron****diffraction**pr**of**ile from LiNiO 2 sample 1. Refinement was donewith the space group for a and b, while the space group C2/mwas used for c.to be R3¯m as has been previously assumed. 18 At the temperaturerange above 335 K, the refinements with the fixed set **of**pr**of**ile parameters produced reasonably good agreements,confirming that the **structure** was essentially R3¯m. However,the agreement deteriorated as the temperature was lowered.Further refining **of** sample-dependent pr**of**ile parameters ateach temperature could bring only partial improvement. Figures2a and 2b show the **neutron**-powder-**diffraction** patternsand their refinements with the R3¯m symmetry at 335and 10 K, respectively. As is easily noticed agreement isquite poor for 10 K. The major source **of** disagreement isanomalous peak broadening for some peaks.Figure 3a shows the temperature-dependent peak broadening**of** the 1 04 reflection, which showed the largestchange with temperature. The anomalous shape **of** the 1 04peak has been reported for room temperature x-ray**diffraction**measurement on Li 0.93 Ni 1.07 O 2 , from which theauthors suggested the existence **of** two phases as an origin **of**the peak broadening. 24 However, in the present study withlow defect concentrations, we can safely rule out this possibilitysince we did not observe extra reflections or linearlyQ-dependent broadening which would implicate the presence**of** a second phase. The systematic peak broadening, as summarizedin Figs. 3b and 3c, was quite different from whatwe would expect from the two-phase behavior. In this plot,064410-3

CHUNG et al.PHYSICAL REVIEW B 71, 064410 2005FIG. 4. Temperature dependence **of** angle deduced from Rietveldrefinement with C2/m model. The meaning **of** the angle isshown in the inset. Closed circles and open squares are fromsamples 1 and 2, respectively. The sold line is a guide to the eyethrough sample 1. The large arrow above the unit cell is the Jahn-Teller-induced shear observed in NaNiO 2 , while the small arrow isthe strain-induced monoclinic shear observed in LiNiO 2 .FIG. 3. a Temperature-dependent peak broadening observedfor the 1 0 4 reflection **of** the **neutron**-**diffraction** pr**of**ile **of**LiNiO 2 . The inset is the comparison between the measured pr**of**ileat 10 K and the calculated one based on C2/m space group. b Thenormalized peak widths **of** the reflections in the **neutron** **diffraction**pr**of**iles **of** LiNiO 2 obtained **by** Gaussian fitting. The obtained peakwidths at each temperature were normalized to the average **of** thosebeyond 400 K. c The slope **of** the temperature-dependent peakwidths as a function **of** the angle between the momentum vector andNiuO bond direction.the width **of** each reflection was normalized to an averagebetween 400 and 585 K, where the peak broadening is negligible.While the peak widths apparently are not systematicallydependent on the magnitude **of** the reciprocal vector Q,they were found to be strongly dependent on its direction.Figure 3c shows the slopes **of** the peak widths, obtained **by**fitting to Fig. 3b between 10 and 350 K and plotted asfunctions **of** the angle that Q makes with the 1 0 3.86reciprocal vector, which is along the three equivalentOuNiuO bonds within the NiO 6 octahedra. The plotshows that the broadening is more pronounced for the reflectionscloser to the orientation **of** the OuNiuO bonds,strongly suggesting relations to the medium-range ordering**of** local Jahn-Teller orbitals. It is certainly inconsistent withrandom orientation **of** local JT distortions, which will resultin anisotropic thermal factors but not in peak broadening.Based on this idea, we tried the Rietveld refinement withthe NaNiO 2 -type C2/m monoclinic model and the result isshown in Fig. 2c. Interestingly, the broadening **of** the peakswas well accommodated into the C2/m **structure**, and a substantiallybetter agreement was achieved. While such monoclinicdistortion is observed for NaNiO 2 which shows collectiveJahn-Teller distortion, 16 this does not imply thehomogeneous NaNiO 2 -type distortion as the ground-state**structure** **of** LiNiO 2 . First, the magnitude **of** the monoclinicshear in LiNiO 2 is smaller than that in NaNiO 2 **by** more thanan order **of** magnitude. More importantly, the sense **of** themonoclinic shear is opposite to that in NaNiO 2 . As a result,the **structure** shows almost no, or inverse, Jahn-Teller distortionswith two NiuO bonds at 1.96 Å and four at 1.97 Å.Figure 4 shows the angle as a measure **of** monoclinic sheardeduced from the C2/m-based Rietveld refinement with thepeak pr**of**ile parameters fixed. It is apparent that below380 K the shear has a small negative linear dependence onthe temperature, but the direction is opposite from what isexpected for the collinear Jahn-Teller distortion. The amount**of** distortion deduced from the Rietveld refinement is assmall as −0.16° at 10 K, compared to +1.98° for NaNiO 2 . 16Therefore, it is apparent that the actual local orbital orderingin LiNiO 2 is dramatically different from the case **of** NaNiO 2 .We note that the obtained as plotted in Fig. 4 may even bean overestimate, and true values may be smaller in magnitude**by** as much as 30%, because we could obtain smaller064410-4

LOCAL STRUCTURE OF LiNiO 2 STUDIED BY…PHYSICAL REVIEW B 71, 064410 2005FIG. 5. The **neutron** pair density functions **of** LiNiO 2 sample 1measured at 10 and 585 K. The x axis for the 585 K data is scaledconsidering the lattice constant expansion. The PDF peaks areclearly seen up to as high as 200 Å.distortions along with better agreement factors **by** fully refiningpeak pr**of**ile parameters under the monoclinic model.In this case, however, we **of**ten found multiple local minimawith similar R factors but with large variance in the obtainedcrystallographic parameters. This ambiguity must be the result**of** having a large number **of** refinable parameters, and wewill not present the result here. The details **of** the peak shapealso argue against the presence **of** a monoclinic unit cell. Theinset in Fig. 3a shows the measured 1 04 reflection at10 K superposed on the refinement with the monoclinicmodel. While the monoclinic model expects unequal weightsfor the split peaks, the measured pr**of**ile does not show a hint**of** a doublet. Therefore, the peak broadening is more consistentwith continuous distributions **of** lattice spacings due tocertain nonuniform distortions than with two different fixedlattice spacings expected in the case **of** monoclinic distortion.We would also like to note that random orientation **of** localJT distortions will not lead to the systematic peak broadeningobserved in the **neutron** **diffraction**. A more plausible explanation**of** this anomalous peak broadening is provided **by** thePDF analysis as described below.B. Pair density functionIn the following, we will discuss the **neutron** pair densityfunction, which provides us with information on the localarrangement **of** Jahn-Teller orbitals. Plots in Fig. 5 show the**neutron** PDFs Gr **of** LiNiO 2 sample 1 directly comparingthe two end temperatures 10 and 585 K. One can immediatelynotice the two most important features in the PDF,which are not directly accessible from **diffraction** patterns.First, the nearest-neighbor peak in the PDF shows a doublepeak**structure** which is a direct confirmation **of** elongatedoctahedra due to local JT distortions. Such a double peak**structure** has been previously observed with extended x-rayabsorption fine **structure** EXAFS, 14,15 but here it is seenwith **diffraction**. However, the result rules out the possibility**of** the orbital frustration recently suggested **by** Reynaud etal. 13 The orbital degeneracy between equally occupiedFIG. 6. The temperature-dependent peak heights obtained fromthe pair density functions Gr **of** LiNiO 2 at a short range, bmedium range, and c long range. The dotted vertical lines aredrawn to highlight the saturation behavior above T=400 K.3d z 2 −r 2 /3 and 3d x 2 −y2 orbitals as suggested **by** them would leadto equal distribution **of** long and short bonds, which is in aclear contradiction with our observation. Our result showsthe weight is approximately 2:1 for short and long NiuObonds, which is consistent with the JT distortion with the3d z 2 −r 2 /3-type orbital that elongates NiO 6 octahedra along thelocal z axis.The most remarkable feature is the inversion **of** PDF peakheights around 80–100 Å. While the short-range peaks below50 Å are taller at lower temperatures reflecting the effect**of** thermal vibration, an opposite, quite unexpected trend isseen for the long-range peaks beyond 100 Å. Figure 6 showsthe temperature dependence **of** several PDF peak heights. Itis clearly seen in Fig. 6c that the peaks beyond 100 Åincrease in height with temperature. A possible interpretation**of** this unusual effect is domain formation at low temperatures,which would lead to a loss **of** medium-range atomiccorrelations. This interpretation is consistent with the broadening**of** the Bragg peaks shown in Fig. 3. We will discussbelow what can possibly induce a temperature-dependent domaineffect. Figure 6 suggests that both short-range andlong-range peaks saturate beyond 400 K. We note that thistemperature is close to the critical temperature found fromthe Rietveld refinement shown in Fig. 4.C. Comparison with similar compoundsConventionally PDFs are used mostly for the study **of**short-range atomic correlations. This, however, is in largepart due to the instrumental Q resolution, as discussed above.The NPDF diffractometer used in this work was designed toallow high-resolution high-intensity **neutron** **diffraction** suitablefor long-range PDF analysis. In order to confirm thiscapability we have compared the PDFs **of** four samples fromthree different compounds with similar triangular symmetry.Plots in Fig. 7 show the ratio between PDF peak heights atlow temperature G LT and at high temperature G HT forLiNiO 2 samples 1 and 2, LiVO 2 and Na 0.75 CoO 2 . The hori-064410-5

LOCAL STRUCTURE OF LiNiO 2 STUDIED BY…PHYSICAL REVIEW B 71, 064410 2005FIG. 8. A possible distortion pattern **of** the randomly orientedJahn-Teller orbitals when there is no c axis bucking **of** the oxygenplane. Thick solid lines show examples **of** possible OuO distancesacross Ni layer, which range from 2.60 to 2.85 Å. The black-greylobes denote the orientations **of** Ni 3+ local 3d z 2 −r 2 /3 orbitals.in Fig. 9. These model **structure**s were refined using the PD-FFIT program 25 to optimize agreement with the measuredPDF. The level **of** agreement was evaluated **by** the R factor,which is the average **of** the square **of** the difference betweenthe model PDF and the measured PDF. The atomic positionsin the model **structure** were improved **by** the least square fitto minimize the R factor. The results are summarized in Fig.10. The average R3¯m **structure** is the one with no local Jahn-Teller distortions. In all other models, the directions **of** thelong OuNiuO axes are depicted with double-sided lobes.Among them the collinear, or the ferro-orbital, correspondsto NaNiO 2 Ref. 16 when the lattice angle parameter deviatesfrom 90°. Other models involve noncollinear ordering**of** local JT distortions **of** the 3d z 2 −r 2 /3 orbitals, with the localz axis varying from site to site. While the zig-zag modelbreaks the threefold symmetry and will result in macroscopicdistortion **of** the lattice, in other noncollinear models the localJT distortions point to all three possible directions withequal weight, and thus will not induce cooperative in-planedistortions.The trimer model shown in Fig. 9, however, has an importantcharacteristic that is not found in the monoclinicferro-orbital or the zig-zag **structure**. Without the JT distortionthree NiO 6 octahedra pointing to three different directionsmay be nicely put together on a plane. However, withJT distortions which elongate some **of** the NiuO distancesthey cannot be accommodated in a flat plane see Fig. 11.Thus the JT distortions are frustrated in this configuration,resulting in further distortion **of** the NiO 2 plane and NiO 6octahedra with all **of** OuNiuO bond angles deviatingfrom 180°. Three long z axes **of** NiO 6 octahedra connect to,and share, an oxygen ion, but this oxygen ion is displacedalong the c axis out **of** the originally flat plane. At the sametime the oxygen ions on the opposite plane shift mainly parallelto the plane. Consequently the NiO 2 plane no longerFIG. 9. An illustration **of** possible short-range ordering **of** Jahn-Teller orbitals that we have tested with PDF refinement. Opencircles denote Ni sites while solid and dashed lines are upper andlower oxygen planes, respectively.retains inversion symmetry. The NiuO distances are splitinto four different bond lengths that naturally fit the shape **of**the nearest-neighbor peak. From the PDF refinement, thelong bonds are found at 2.04 and 2.06 Å while the shortbonds are at 1.90 and 1.96 Å, so the average lengths for longand short NiuO bonds are 2.05 and 1.93 Å, respectively.The bond lengths from the C2/m model were found atslightly shorter distances **of** 2.04 and 1.91 Å, respectively.The amount **of** JT distortion estimated from this study is a bitsmaller than the result **of** an ab initio calculation, 26 but closeto what was estimated from EXAFS measurement. 14 The fittingrange as shown in Fig. 10 is up to 5.2 Å, which isslightly larger than the size **of** one trimer unit. We note thatthe intensity around 3.5 Å is smaller for all the models comparedto the experimental PDF. This systematic deviationappears to be due to experimental errors, most likely relatedto the correction for inelastic intensities.The results summarized in Fig. 10 show that the averageR3¯m model fairly well reproduces the features beyond thefirst peak, but badly fails to describe the JT split **of** the firstpeak. While the PDF **of** other models we have tried obviouslydo not reproduce the measured PDF, apparently theagreements were the best for the monoclinic C2/m and the064410-7

CHUNG et al.PHYSICAL REVIEW B 71, 064410 2005FIG. 11. a A lateral view **of** a single NiO 2 slab. Double-sidedlobes are Ni 3d z 2 −r 2 /3 orbitals with long NiuO bonds, and emptycircles are oxygen sites. For either oxygen or nickel site, thosecloser or farther from the viewer are represented **by** relative sizes.For Ni 3+ orbitals, black and gray lobes denote closer and fartherpositions, respectively. b A lateral view **of** a stack **of** multipleslabs. The arrows indicate the direction **of** monoclinic shear. Thedotted line is the domain boundary, beyond which the curvaturereverses.trimer models. The asymmetric shape **of** the first peak isclosely reproduced **by** both models. The trimer models showa better agreement for the OuO correlations around 3 Å,while the monoclinic model does better for the slightlylonger range. In the case **of** the monoclinic model, however,the comparison with the Rietveld refinement suggests that itis not likely the true local **structure**. While the cooperativein-plane shift **of** the oxygen layers conveniently reproducedthe JT split, this shift badly failed to realize in the Rietveldrefinement. Compared to the NaNiO 2 **structure**, the collinearmodel shown in Fig. 10 has the oxygen ion pushing againstthe Li site, under which situation the negative monoclinicshear is unlikely see Fig. 4. The unlikeliness **of** such uniformshift is also reflected in a relatively poor agreement **of**the OuO correlation peaks between 2.6 and 3.2 Å. Therefore,the monoclinic collinear **structure** obtained **by** the PDFrefinement is supposed to be an accidental one. We alsostress that the ferro-orbital arrangement is inconsistent withobserved magnetic properties **of** LiNiO 2 , which is in clearcontrast with that **of** NaNiO 2 .All these points and a relatively large R factor make themonoclinic **structure** less favorable than the trimer models.Thus, it is most likely that the trimer models are the actualshort-to-medium range **structure**. Unfortunately, the reciprocalspace Rietveld refinement with the trimer models are notpossible, since the superlattice peaks due to the orbital orderingare mostly very weak in intensity. We need a single crystal**diffraction** study to detect these superlattice peaks. In thefollowing, we will present more arguments why the trimer**structure**s are most likely the true local **structure**, and amongthem, the fully ordered trimer **structure** must be the groundstate **structure**.FIG. 10. Results **of** short-range pair density function refinementswith several tried models. The crosses are the measured PDF at10 K, and the solid and dash-dotted lines are the calculated PDFand its difference from the data, respectively. The R factors areshown in the plots.B. Origin **of** the limited correlation lengthWe have mentioned above that the JT distortion is locallyfrustrated in the trimer ordering model, which results in thedistortion **of** the NiO 6 octahedra. We now discuss the impli-064410-8

LOCAL STRUCTURE OF LiNiO 2 STUDIED BY…cation **of** this local distortion to the long-range order. Thetrimer ordering **of** JT distortion induces displacement **of** theoxygen ion shared **by** three JT distorted octahedra out **of** theplane, and stresses between oxygen ions. At the same time,the three other long NiuO bonds pointing towards the oppositeplane push the oxygen ions sideways, creating a compressivestress against surrounding oxygen ions see Fig.11a. As a result, the NiO 2 slab becomes slightly curved.Since the curved slab is inconsistent with the average **structure**,this results in yet another level **of** frustration, and preventsthe trimer ordering from becoming the long-range order.Therefore it is reasonable to assume that domains will beformed consequently to accommodate the curvature. Thecurving **of** the layer will be correlated along the c axis Fig.11b, producing three-dimensional domains. In a perfect**structure** domains will be regular and periodic, but any defectscould pin them, and make them random. Thus the structuralcoherence is likely to be limited **by** the domain size.This explains quite well the observed crossover behavior **of**the PDF shown in Fig. 7 and the Bragg peak broadeningshown in Fig. 3b. As shown in Fig. 7 two samples withdifferent defect densities have different crossover points,suggesting different domain sizes. This supports our viewthat the domains are pinned **by** defects. However, as mentionedearlier the fact that sample 1 has a smaller domainsuggests that pinning does not occur at the domain walls. Itis more likely that defects allow larger deformation and alarger domain size. On the other hand, the alternating trimermodel corresponds to the trimer model with a narrow onedimensionaldomain with alternating curvature. This modeldoes not lead to the nanoscale frustration, and does not explainthe domain formation and the crossover phenomenonin Fig. 7.It should be pointed out that the Bragg peak broadeningshown in Fig. 3 should not be directly interpreted in terms **of**the structural coherence length. It more strongly reflects thedistribution **of** lattice spacings induced **by** the monocliniclikedistortion. Since the shear stress tensor has a center **of** symmetryat the center **of** the domain, the domain cannot have amonoclinic symmetry as a whole. This also explains why wedo not observe a monoclinic peak splitting, which otherwiseis expected as shown in the inset **of** Fig. 3a. We emphasizethat such a bent slab will not disturb the lattice spacings **of**0 0l or h k0 planes very much. On the other hand, forthe planes nearly perpendicular to the orientation **of** 3d z 2 −r 2 /3Jahn-Teller orbitals, the monoclinic shear will certainly havelarger effects. Indeed the peak width is strongly correlatedwith the angle away from the NiO 4 square basal plane **of** theJT distorted NiO 6 octahedron, as shown in Fig. 3c. Therefore,we can conclude that the average **structure** **of** LiNiO 2 isstill hexagonal even at low temperatures, and the monoclinicitysuggested in the **diffraction** pr**of**iles is simply a reflection**of** the local stress effect.We note that the changes in the powder **diffraction** peakwidths Fig. 3b, in the PDF peak heights see Fig. 6cand the monoclinic distortion all take place at T d =375 K.Therefore, it is likely that this temperature is where the trimerordering begins and distorts the local as well as globallattice **structure**. We note again that this temperature is veryclose to the temperature where the dc susceptibility anomalyPHYSICAL REVIEW B 71, 064410 2005was observed and interpreted in terms **of** the orbital exchangeinteraction. 13C. Discussions on possible implication to magnetismTo understand the magnetic properties **of** LiNiO 2 it is importantto make measurements on samples with the leastamounts **of** defects, on which their properties are stronglydependent. 7,9,24 The most prevalent type **of** defect is believedto be Ni substitution **of** Li ions. Such substitution can introduceinterplanar ferromagnetic coupling between Ni layers.This interplanar exchange is supposed to be stronger than theintraplanar one since the NiuOuNi bond angle for an interplanarNi pair through substitutional Ni is nearly 180°,while that **of** an intraplanar one is close to 90°. With low Niimpurity concentrations x0.02, however, the ferromagneticcoupling is weak and the material shows a tendency for antiferromagneticfluctuations. 24 For the near-stroichiometriccomposition, the intraplanar exchange must be the primarycomponent **of** the magnetic coupling, and the orbital orderingis expected to play an important role. While magnetic measurementsmay be masked **by** small amounts **of** impurity, theorbital-lattice interaction should certainly be observable. Thecomparison between the two samples in our study suggestsnot only that the proposed orbital ordering is very likely tobe intrinsic, but also that it persist up to moderate impurityconcentrations.What is particularly interesting is the obvious differencebetween NaNiO 2 and LiNiO 2 . In the case **of** NaNiO 2 ,3d z 2 −r 2 /3 orbital orientation is collinear and the intraplanarexchange is ferromagnetic, while the interplanar exchange isantiferromagnetic. 17 According to the Kanamori-Goodenough rule the 90° exchange can lead to ferro-orbitalordering via the spin-orbit decoupling when the Hund couplingbetween oxygen holes is negligible. On the other hand,the situation **of** LiNiO 2 is distinctly unclear. Experimentallya tendency for antiferromagnetic orbital fluctuations isobserved, 4–7 which would imply triangular symmetry betweenneighboring orbitals is favored. However, no apparentlong-range ordering has been found in LiNiO 2 . It has beenspeculated that the quantum spin-orbital liquid state may beformed via orbital degeneracy, 27 but our result clearly showsthat the orbital order is not in a liquid state. Mostovoy et al. 28attributed the absence **of** orbital ordering in LiNiO 2 to animpurity effect, while our analysis argues against it. Althoughthe effect **of** impurity is apparent in LiNiO 2 , our resultsdo not point to ferro-orbital ordering as an intrinsiclimit, but suggest a completely different kind **of** orbital ordering,involving trimer local ordering **of** orbitals.Interestingly, the trimer model provides a possible interpretationfor the coexistence **of** ferromagnetic and antiferromagneticspin fluctuations without considering an impurityeffect. The three 3d z 2 −r 2 /3 orbitals forming a trimer couldform a spin-singlet state if the nearest-neighbor exchangeamong them is negative. While the Goodenough-Kanamori-Anderson rules suggest a positive exchange, the trigonalcrystal-field effect at the oxygen site could result in an antiferromagneticexchange, as pointed out recently. 29 On thetwo-dimensional plain, there are two choices how the trimer064410-9

CHUNG et al.units can be arranged as shown on the bottom part **of** Fig. 9.In the basic trimer model, the units again retain triangularsymmetry, subject to geometrical fluctuations at the trimercluster level. On the other hand, the alternating trimer modelloses the triangular symmetry, so that we cannot rule out thepossibility **of** short-range magnetic ordering that lifts geometricalfrustration within the trimer. It is most likely that thetriangular arrangement **of** trimers prevails in the bulk **of** thesystem domain with curved plane, and the alternating patternis found at the boundary between the domains. A recentsuggestion on the presence **of** ferromagnetic clusters withinthe plane 30 could be attributed to such a domain boundaryeffect. We suspect that this domain boundary can restrict theextent **of** antiferromagnetic fluctuations, effectively reducingpossible consequences **of** quantum fluctuations. The curvedlattice in the trimer model implies another interesting complicationin achieving a stable ground state. Since one domainwith a positive curvature has to be contiguous to anotherdomain with a negative curvature, the triangularsymmetry again leads to a morphological frustration betweenthree neighboring domains similarly to magnetic frustration.In the presence **of** impurities, which may pin the domainwalls, the configuration **of** the frustrated domains will beirregular. We suspect that LiNiO 2 is a system where its macroscopicphysical properties are determined **by** several layers**of** coexisting atomic–short-range–intermediate-range frustrations.The frustrated domains may lead to interesting elasticproperties, which should be detectable **by** a careful measurementon the elastic tensor **of** a single crystal.V. CONCLUSIONSWe have performed a temperature-dependent **neutron** **diffraction**study **of** LiNiO 2 in order to probe the local ordering**of** Ni 3+ Jahn-Teller orbitals. From the combined analysis **of**the real space pair distribution function and the reciprocalPHYSICAL REVIEW B 71, 064410 2005space **diffraction** pr**of**ile, we conclude that the JT distortionsin this material are not randomly oriented, but form localordering. The ordering is quite different from the collineartype found in NaNiO 2 , and is most likely the trimer type,where three 3d z 2 −r 2 /3 orbitals point towards the shared oxygensite. In this model, the shared oxygen site will be displacedaway from the NiO 2 plane, forcing the NiO 2 plane tohave a curvature. Since the neighboring planes will have asimilar curvature and the curvature prevents the trimer orderingfrom becoming long-range order, the system is composed**of** nanoscale domains **of** local trimer order. A signature **of**such a curved plate can be found in the **diffraction** pr**of**ile asthe monocliniclike peak broadening. The temperature for theshort-range trimer ordering to take place is estimated to be375 K. The unconventional magnetism observed in thismaterial may be explained in the context **of** the interplaybetween Ni 3+ 3d z 2 −r 2 /3 orbitals, trimer units, and domains undera triangular symmetry.ACKNOWLEDGMENTSThe authors thank D. Khomskii, A. R. Bishop, A. Saxena,A. Stepanov, and R. Hayn for useful discussions. This workwas supported **by** the National Science Foundation throughGrant No. DMR01-02565 and **by** the Laboratory DirectedResearch and Development Program **of** Oak Ridge NationalLaboratory, managed **by** UT-Battelle, LLC, for the U.S. Department**of** Energy under Contract No. DE-AC05-00OR22725. This work has benefited from the use **of** NPDFat the Lujan Center at Los Alamos Neutron Science Center,funded **by** DOE Office **of** Basic Energy Sciences and LosAlamos National Laboratory funded **by** Department **of** Energyunder Contract No. W-7405-ENG-36. The upgrade **of**NPDF has been funded **by** NSF through Grant No. DMR00-76488.*Present address: NIST Center for Neutron Research, National Institute**of** Standard and Technology, Gaithersburg, MD 20899,USA and University **of** Maryland, College Park, Maryland 20742,USA.1 K. Hirakawa, R. Osborn, A. D. Taylor, and K. Takeda, J. Phys.Soc. Jpn. 59, 3081 1990.2 P. W. Anderson, Mater. Res. Bull. 8, 153 1973.3 J. P. Kemp, P. A. Cox, and J. W. Hod**by**, J. Phys.: Condens.Matter 2, 6699 1990.4 H. Yoshizawa, H. Mori, K. Hirota, and M. Ishikawa, J. Phys. Soc.Jpn. 59, 2631 1990.5 K. Hirota, Y. Nakazawa, and M. Ishikawa, J. Phys.: Condens.Matter 3, 4721 1991.6 A. Rougier, C. Delmas, and G. Chouteau, J. Phys. Chem. Solids57, 1101 1996.7 A.-L. Barra, G. Chouteau, A. Stephanov, and C. Delmas, J.Magn. Magn. Mater. 177–181, 783 1998.8 J. N. Reimers, J. R. Dahn, J. E. Greendan, C. V. Stager, G. Liu, I.Davidson, and U. von Sacken, J. Solid State Chem. 102, 5421993.9 K. Yamaura, M. Takano, A. Hirano, and R. Kanno, J. Solid StateChem. 127, 109 1996.10 M. Corti, S. Marini, A. Rigamonti, V. Massarotti, and D. Capsoni,J. Appl. Phys. 79, 6621 1996.11 A. Bajpai and A. Banerjee, Phys. Rev. B 55, 12 439 1997.12 Y. Kitaoka, T. Kobayashi, A. Koda, H. Wakabayashi, Y. Nino, H.Yamakage, S. Taguchi, K. Amaya, K. Yamaura, M. Takano, A.Hirano, and R. Kanno, J. Phys. Soc. Jpn. 67, 3703 1998.13 F. Reynaud, D. Mertz, F. Celestini, J.-M. Debierre, A. M. Ghorayeb,P. Simon, A. Stepanov, J. Voiron, and C. Delmas, Phys.Rev. Lett. 86, 3638 2001.14 A. Rougier, C. Delmas, and A. V. Chadwick, Solid StateCommun. 94, 123 1995.15 I. Nakai, K. Takahashi, Y. Shiraishi, T. Nakagome, and F. Nishikawa,J. Solid State Chem. 140, 145 1998.16 L. D. Dyer, B. S. Borie, Jr., and G. P. Smith, J. Am. Chem. Soc.76, 1499 1954.17 P. F. Bongers and U. Enz, Solid State Commun. 4, 153 1966.064410-10

LOCAL STRUCTURE OF LiNiO 2 STUDIED BY…18 C. Pouillerie, E. Suard, and C. Delmas, J. Solid State Chem. 158,187 2001.19 V. Bianchi, D. Caurant, N. Baffier, C. Belhomme, E. Chappel, G.Chouteau, S. Bach, J. P. Pereira-Ramos, A. Sulpice, and P. Wilmann,Solid State Ionics 140, 12001.20 Th. Pr**of**fen, T. Egami, S. J. L. Billinge, A. K. Cheetham, D.Louca, and J. B. Parise, Appl. Phys. A: Mater. Sci. Process. 74,S163 2002.21 A. Larson and R. B. von Dreele, GSAS: General Structure AnalysisSystem, Los Alamos National Laboratory, 1994.22 T. Egami and S. J. L. Billinge, Underneath the Bragg Peaks:Structural Analysis **of** Complex Materials Pergamon, Amsterdam,2003.23 P. F. Peterson, M. Gutmann, Th. Pr**of**fen, and S. J. L. Billinge, J.Appl. Crystallogr. 33, 1192 2000.PHYSICAL REVIEW B 71, 064410 200524 F. Reynaud, A. M. Ghorayeb, Y. Ksari, N. Menguy, A. Stephanov,and C. Delmas, Eur. Phys. J.: Appl. Phys. 14, 832000.25 Th. Pr**of**fen and S. J. L. Billinge, J. Appl. Crystallogr. 32, 5721999.26 C. A. Marianetti, D. Morgan, and G. Ceder, Phys. Rev. B 63,224304 2001.27 L. F. Feiner, A. M. Oles, and J. Zaanen, Phys. Rev. Lett. 78, 27991997.28 M. V. Mostovoy and D. I. Khomskii, Phys. Rev. Lett. 89, 2272032002.29 A.-M. Dar, R. Hayn, and J.-L. Richard, Europhys. Lett. 61, 8032003.30 J. van Duijn, B. Gaulin, S. Park, S.-H. Lee, and J. Copley, Bull.Am. Phys. Soc. 48, N31.006 2003.064410-11